**HAL Id: tel-03272250**

**https://pastel.archives-ouvertes.fr/tel-03272250**

Submitted on 28 Jun 2021
**HAL is a multi-disciplinary open access**
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

**Probabilistic single fibre characterisation to improve**

**stochastic strength modelling of unidirectional**

**composites**

### Faisal Islam

**To cite this version:**

### Pr ´epar ´ee `a MINES ParisTech

**EN: Probabilistic single fibre characterisation to improve**

**stochastic strength modelling of unidirectional composites**

**FR: Caract ´erisation probabiliste monofilamentaire pour**

**am ´eliorer la mod ´elisation stochastique de la r ´esistance des**

**composites unidirectionelles**

Soutenue par
**Faisal ISLAM**

Le 3 juin 2020
´
Ecole doctorale no_{621}

**Ing ´enierie des Syst `emes,**

**Mat ´eriaux, M ´ecanique,**

**Energ ´etique**

Sp ´ecialit ´e

**M ´ecanique**

Composition of the jury : Peter DAVIES

Ing ´enieur de Recherche, IFREMER Rapporteur Vincent PLACET

Ing ´enieur de Recherche, Universit ´e de Franche-Comt ´e

Rapporteur V ´eronique MICHAUD

Associate Professor, EPFL Examinateur James THOMASON

Professor, University of Strathclyde Examinateur Nicolas SAINTIER

Professor des Universit ´es, ENSAM I2M Pr ´esident S ´ebastien JOANN `ES

Charg ´e de Recherche, Mines ParisTech Examinateur Lucien LAIARINANDRASANA

Directeur de recherche,

**Acknowledgements**

I would like to express my sincere gratitude to my supervisors Dr. S´ebastien Joann`es and Prof. Lucien Laiarinandrasana for their support, guidance and numerous interesting discussions throughout this PhD project. I am also very grateful to Dr. Anthony Bunsell and Dr. Alain Thionnet for sharing their knowledge and scientific advice and for the many insightful suggestions during my interactions with them.

I would like to acknowledge the funding from the European Union’s Horizon 2020 re-search and innovation programme under the Marie Sklodowska-Curie grant agreement No. 722626 (FibreMod, www.fibremodproject.eu) for supporting my research and the several professional trainings received during my PhD. which provided me with incompa-rable opportunities for career development in an international environment ranging across different continents.

A particular thanks to the technical staff of the Materials Centre of Ecole des Mines de Paris: especially Julie and Jean-Christophe who have greatly contributed with their expertise to the success of a major part of the work produced in this PhD, embarking with enthusiasm and success on technical challenges never faced before. Thanks to Zak for all his help with administrative tasks.

I would like to thank my closest collaborators from Dia-Stron Ltd.: Dr. Steve Bucknell and Yann Leray; from Weizmann Institute of Science: Prof. Daniel Wagner and Carol Rodricks; and from Chomarat Ltd.: Dr. Vicky Singery and Dr. Ashok Rajpurohit for the fruitful research and collaborations we had during the years of my PhD. Additionally, a very important thanks goes to all the FiBreMoD project partners and PhD students for the challenging discussions and professional growth opportunities that the several consortium meetings and project events have provided. The FiBreMoD early stage researchers deserve a special mention for their support and the collective effort we put into reaching the milestones of the project.

I would like to thank all the members of the Materials Centre and the many other colleagues and friends that I have met and collaborated with at Ecole des Mines of Paris. Thanks for having a very productive environment for research and for always being so helpful and friendly. I would also like to thank all members of the examination committee for their feedback during the interim presentations and their corrections of this manuscript. I would like to thank my friends, and colleagues Jan Rojek, Martinus and Ashok Rajpuro-hit who shared with me, day-by-day, pains and glories of this PhD and of these three years in France. A special thanks goes to my old friends from India: Atul, Aaquib, Nadeem

2

and Shaheer with whom I kept good friendships despite the distance and the different professional paths undertaken over the years.

Again, I will forever be thankful to S´ebastien for all his help in many different academic and non-academic ways. His help in all practical aspects is deeply appreciated. He has been my role model as a scientist, mentor, and supervisor.

**Contents**

Acknowledgements . . . 1

List of publications . . . 13

**Preamble** **15**
Background and Motivation . . . 15

Aim . . . 15

Thesis as part of the FiBreMoD project . . . 16

**1** **Introduction** **17**
1.1 Structural applications of fibre reinforced composites . . . 17

1.2 Predictive models for fibre composites . . . 18

1.2.1 Issues with model predictions . . . 18

1.3 Constituent properties: Input data for models . . . 19

1.3.1 Fibre strength . . . 20

1.3.2 Matrix and interfacial properties . . . 22

1.4 Main objectives of the thesis . . . 23

1.5 Thesis outline . . . 24

Chapter summary in French . . . 26

**2** **Fibre strength and Weibull distribution: state-of-the-art** **29**
2.1 Introduction . . . 29

2.1.1 Fibres used in composite materials . . . 30

2.2 Fibre strength . . . 31

2.2.1 Weakest link model for fibre strength . . . 31

2.2.2 Representation of fibre strength with Weibull distribution . . . 32

2.2.3 Physical interpretation of Weibull distribution parameters . . . 33

2.3 Fibre strength characterisation . . . 33

2.3.1 Fibre bundle test . . . 35

2.3.2 Fragmentation test . . . 36

2.3.3 Loop test . . . 37

2.3.4 Single fibre test . . . 38

2.3.5 Estimation of Weibull parameters from fibre strength data set . . . . 40

2.4 Issues in determining fibre strength . . . 41

2.5 Issues with the standard Weibull distribution . . . 42

2.5.1 Extrapolation of distribution parameters . . . 42

4 CONTENTS

2.5.3 Uncertainty in results . . . 43

2.6 Conclusions . . . 44

Chapter summary in French . . . 46

**3** **Critical parameters in fibre strength measurement: identification and**
**evaluation** **47**
3.1 Introduction . . . 49

3.2 Critical parameters in fibre strength measurement . . . 50

3.2.1 Sources of uncertainty . . . 50

3.2.2 Fibre tensile strength : Theoretical formulation . . . 50

3.2.3 Measurement uncertainty . . . 54

3.2.4 Experimentation . . . 55

3.2.5 Evaluation of measurement uncertainty in input quantities . . . 56

3.2.6 Propagation of uncertainty to fibre tensile strength . . . 58

3.3 Sensitivity analysis . . . 61

3.3.1 Sensitivity analysis for fibre tensile strength . . . 62

3.3.2 Estimation of sensitivity for tensile strength at other gauge lengths 63 3.4 Conclusions . . . 64

Chapter summary in French . . . 67

**4** **Uncertainty in fibre strength distribution** **69**
4.1 Introduction . . . 71

4.1.1 Causes of uncertainty in Weibull parameters . . . 71

4.2 Uncertainty due to measurement . . . 72

4.2.1 Fibre strength distribution . . . 73

4.2.2 Estimation of measurement uncertainty on Weibull parameters . . . 74

4.3 Uncertainty due to sampling randomness . . . 76

4.3.1 Confidence Interval . . . 77

4.3.2 Calculation of confidence interval for Weibull parameters . . . 77

4.3.3 Confidence Region . . . 81

4.3.4 Effect of sample size . . . 82

4.4 Conclusions . . . 83

Chapter summary in French . . . 85

**5** **Variability in predictions of composite strength models due to uncertain**
**input properties** **87**
5.1 Introduction . . . 89

5.2 Mines ParisTech model . . . 89

5.2.1 Mechanism of longitudinal tensile failure of unidirectional composites 90 5.2.2 Microscopic scale: Fibre failure model and the RVE . . . 90

*5.2.3 Macroscopic analysis: Simplified FE*2 _{model . . . 91}

5.3 Methods . . . 91

5.3.1 Steps in simulation . . . 91

5.3.2 Simulation framework . . . 93

5.3.3 Input fibre strength: Hypothetical properties with uncertainties . . . 94

5.3.4 Loading conditions . . . 95

CONTENTS 5

5.4.1 Monotonic loading . . . 97

5.4.2 Sustained loading . . . 100

5.5 Conclusions . . . 102

Chapter summary in French . . . 104

**6** **Experimental and statistical investigation of fibre properties** **107**
6.1 Introduction . . . 109

6.2 Material and methods . . . 110

6.2.1 Material . . . 110

6.2.2 Methods . . . 110

6.2.3 Advantages of using the semi-automated testing method . . . 114

6.3 Experimentation . . . 116

6.3.1 Fibre dimensional measurement . . . 116

6.3.2 Fibre tensile strength measurement . . . 118

6.4 Results and discussions . . . 118

6.4.1 Fibre dimensional analysis . . . 118

6.4.2 Measurement of Poisson’s ratio . . . 121

6.4.3 Tensile strength . . . 124

6.4.4 Strength distribution . . . 127

6.4.5 Effect of sample size on the confidence interval . . . 131

6.5 Conclusions . . . 132

6.5.1 Scope for improvement in the fibre testing system . . . 135

Chapter summary in French . . . 136

**7** **Weibull analysis based on Bayesian approach** **137**
7.1 Introduction . . . 139

7.2 Cause of misfit: Fibre preselection effect . . . 140

7.2.1 Fibre preselection effect . . . 140

7.2.2 Simulated experiment for demonstrating fibre preselection effect . . 140

7.2.3 Need for improvements in analysis . . . 143

7.3 Truncated Weibull analysis based on Bayesian approach . . . 143

7.3.1 Existence of truncation in fibre strength data . . . 143

7.3.2 Theoretical formulation . . . 144

7.4 Experiments, Results and Discussions . . . 147

7.4.1 Experimentation . . . 147

7.4.2 Fibre strength results . . . 147

7.4.3 Standard Weibull analysis . . . 147

7.4.4 Truncated Weibull analysis . . . 150

7.5 Conclusions . . . 153

Chapter summary in French . . . 154

**8** **Conclusions and perspectives** **155**
8.1 Conclusions . . . 155

8.2 Perspectives . . . 157

8.2.1 Limitations of extrapolating fibre strength . . . 157

8.2.2 Modification of Weibull distributions . . . 158

6 CONTENTS

Chapter summary in French . . . 162

**A** **Weakest link model and Weibull distribution** **175**
**B Microscale matrix properties** **177**
B.1 Introduction . . . 177

B.2 Microscale matrix properties: state of the art . . . 178

B.3 Materials and methods . . . 180

B.3.1 Materials . . . 180

B.3.2 Specimen preparation . . . 180

**List of Figures**

1.1 Some structural applications of fibre reinforced composite materials. . . 18 1.2 Weibull parameter values for T700 carbon fibres reported in literature . . . 22 2.1 Rovings of different fibre types used in composite materials. . . 31 2.2 Schematic representation of a chain consisting of N links. . . 32 2.3 Effects of the shape, scale and location parameters on Weibull distribution. 34 2.4 Schematic view of the initial part of the load-strain curve for a bundle test 35 2.5 Schematic of a specimen for a single fibre fragmentation test . . . 36 2.6 Schematic of a single fibre loop test. . . 38 2.7 Schematic of a single fibre mounted on a card frame . . . 39 3.1 (a) Schematic diagram of a single fibre mounted on a card frame, (b) Major

issues with sample preparation leading to inaccurate measurement of gauge length, (c) Angular misalignment in the fibre specimen . . . 51 3.2 Schematic diagram showing the effect of fibre misalignment on the effective

load on the fibre. . . 52 3.3 The actual card frame used for preparing the fibre specimens. . . 55 3.4 Failure stress vs failure strain scatterplot for all fibre tensile tests . . . 61 3.5 Sensitivity indices of different input quantities in tensile strength

measure-ment of fibres at different gauge lengths . . . 65 4.1 Estimated Weibull plot for experimentally determined fibre strength . . . . 73 4.2 Weibull distributions simulated by varying fibre strength data points within

the uncertainty region . . . 75 4.3 Simulated Weibull distributions based on sampling and measurement

un-certainty. . . 79 4.4 Simulated fibre strength data sets. . . 80 4.5 Scatter between the shape and scale paramaters of the simulated Weibull

distributions. . . 80 5.1 Representative Volume Element at the microscopic scale with the fibres

distributed in a regular square array. . . 91 5.2 RVEs of the material damage state resulting from sequential fibre breaks

and corresponding i-plets. . . 92
*5.3 Flowchart of the simplified F E*2 _{multiscale fibre break model. . . 92}

8 LIST OF FIGURES 5.4 (a) Specimen of dimensions 64 mm × 4 mm × 1 mm. (b) A C3D8 linear

3-D brick element consisting of 8 RVEs. (c) An RVE with 32 fibres . . . 94 5.5 Characteristic curves for the monotonic loading condition . . . 96 5.6 Characteristic curves for the sustained loading condition . . . 97 5.7 Simulated composite behaviour for different input fibre strength

distribu-tions with varying scale parameters. . . 98 5.8 Simulated composite behaviour for different input fibre strength

distribu-tions with varying shape parameters. . . 99 5.9 Simulated composite behaviour for different input fibre strength

distribu-tions with varying scale parameters, under the sustained loading condition. 100 5.10 Simulated composite behaviour for different input fibre strength

distribu-tions with varying shape parameters, under the sustained loading condition. 102 6.1 (a) Dia-Stron Fibre Dimensional Analysis System (FDAS770, Isometric

view). (b) Working of the FDAS770 (top view). (c) Zoomed-in image of the translation stage. . . 111 6.2 (a) Plastic tabs used for mounting one end of a fibre. (b) Well defined gauge

length with proper alignment. . . 112 6.3 A 20 sample cassette loaded with fibre specimens ready to be tested. . . 113 6.4 (a) ALS Vacuum suction for specimen pick up (b) transfer of specimen to

testing site. . . 113 6.5 (a) Testing site: Combination of the LEX/LDS system. (b) Testing setup

installed with the LEX/LDS system. . . 114 6.6 Schematic diagram of unwrapping a fibre surface on a 2-D plane to show

the different locations at which dimensional measurements were recorded. . 117 6.7 Histograms showing the variations in measured fibre diameters for all fibres

*of the different gauge lengths: (a) L*0*=30 mm, (b) L*0*=20 mm, (c) L*0=4 mm119

6.8 Variation in apparent fibre diameter along the axial length for different angular positions: (a) for Fibre 1. (b) for Fibre 2 . . . 120 6.9 Variation in measured fibre diameter along the angular direction, for a fixed

plane (apparent cross-section), for: (a) fibre 1 (b) fibre 2. Unit: micrometres.121 6.10 Schematic of the change in axial and lateral dimensions of the fibre on

elongation. . . 122 6.11 Reduction in measured fibre diameter with elongation. . . 123 6.12 Boxplots for fibre strengths for the three gauge lengths with mean and

median values . . . 124 6.13 Fibre strength plotted against failure stress for all fibres, along with

corre-sponding histograms, for tensile tests done at gauge lengths of 30 mm. The straight line represents the mean Young’s modulus. . . 126 6.14 Fibre strength plotted against failure stress for all fibres, along with

corre-sponding histograms, for tensile tests done at gauge lengths of 20 mm. The straight line represents the mean Young’s modulus . . . 126 6.15 Fibre strength plotted against failure stress for all fibres, along with

LIST OF FIGURES 9 6.16 Fibre strength plotted against fibre diameter for all fibres, for tensile tests

done at all the different gauge lengths . . . 128 6.17 Best fit Weibull plots for the 2-parameter distribution for all three gauge

lengths, along with experimental data points . . . 129 6.18 Best fit Weibull plots for the 3-parameter distribution for all three gauge

lengths . . . 131 6.19 Simulated fibre strength data sets. . . 133 7.1 Distribution used for determining the break limit for individual fibre strength

values. It is a folded normal distribution with a mean of 2 GPa and a stan-dard deviation of 0.5 GPa. . . 142 7.2 Weibull plot showing simulated fibre strength data for a Weibull distribution

*with σ*0*=4.5 GPa and m = 4.0, along with the fibre strength data set after*

simulating the fibre preselection effect. . . 142
*7.3 Relationship between location parameter (σu) and truncation limit (σr*) for

*different cases. (a) Case 1: σu* *= 0 (b) Case 2: 0 < σu* *< σr* (c) Case 3:
*σu* *= σr* . . . 144

7.4 Histogram of the experimentally generated fibre strength data. . . 148 7.5 Best representative standard 2 and 3-parameter Weibull distributions along

with experimental fibre strength data. . . 149 7.6 Truncated and predicted Weibull distributions for the three cases. . . 151 8.1 Comparison of the scale parameters obtained from extrapolation with that

obtained from experimental results. . . 158 A.1 Schematic representation of a chain consisting of N links. . . 175 B.1 (a) Fibre manufacturing process used by Hobbiebrunken et al. (b) Fibre

manufacturing process used by Misumi et al. . . 179 B.2 Cross-section of a carbon fibre reinforced composite material. The epoxy

phase can be seen to have non-regular shapes. . . 180 B.3 Schematic of the cross section of the group of wires. The epoxy settled in

the cavities near the point of contact of consecutive wires resulting in epoxy fibres. . . 181 B.4 An epoxy fibre. The fibre is twisted along the length due to the twists given

to the teflon wires for consolidation. . . 181 B.5 Microscopic image of the cross-section of the wires with epoxy settled in

**List of Tables**

1.1 Weibull distribution parameters for T700 carbon fibres reported in
*litera-ture. The scale parameter (σ*0*) normalized for L*0 = 30 mm. ‘SFT’ stands

for single fibre tests, ‘Fragm.’ stands for fibre fragmentation tests, and ‘Bundle’ stands for fibre bundle tests. . . 21 3.1 Best estimate values of all quantities for one single fibre tensile test . . . 56 3.2 Measurement uncertainty values of all input quantities for the given fibre

tensile test example, along with expanded uncertainty for a confidence level of 95% and 99%. . . 58 3.3 Sensitivity coefficient values of all quantities . . . 60 3.4 Best estimates and measurement uncertainty of fibre strength for 30 tensile

tests . . . 61 3.5 Sensitivity measures of each input quantity for the given single fibre tensile

test example . . . 62 3.6 Average sensitivity measures for each input quantity for the set of 30 single

fibre tensile test . . . 63 3.7 Sensitivity indices of different input quantities in tensile strength

measure-ment of fibres at different gauge lengths . . . 64 4.1 Weibull parameters for experimentally determined fibre strengths . . . 73 4.2 Weibull parameters for virtual fibre strength data sets . . . 75 4.3 Amplification of measurement uncertainties of the Weibull Scale

*parame-ter (σ*0) upon extrapolation to shorter gauge lengths. . . 76

4.4 Weibull parameters and associated 95% confidence interval for overall un-certainty due to measurement and sampling. . . 79 4.5 Amplification of uncertainties (due to sampling randomness) of the Weibull

*Scale parameter (σ*0) upon extrapolation to shorter gauge lengths. . . 81

4.6 Best estimated values for selective B-strengths along with the 95% confi-dence intervals for overall uncertainty due to measurement and sampling . . 83 4.7 Effect of sample size on estimated 95% confidence interval of Weibull scale

*parameter σ*0 (B63.2 strength) . . . 83

5.1 Elastic properties of an undamaged UD ply for 64% fibre volume fraction. . 94 5.2 Different levels of the shape and scale parameters of the input fibre strength

12 LIST OF TABLES 5.3 Simulated failure stress values of the composite for input fibre strength

distributions having different scale parameters and same shape parameter . 98 5.4 Simulated failure stress values of the composite for input fibre strength

distributions having different shape parameters and same scale parameter . 99 5.5 Simulated lifetime of the composite structure for input fibre strength

dis-tributions having different scale parameters and same shape parameter . . . 101

5.6 Simulated lifetime of the composite structure for input fibre strength dis-tributions having different shape parameters and same scale parameter . . . 101

6.1 Fibre properties supplied by the manufacturer . . . 110

6.2 Comparison of semi-automated and standard manual single fibre testing methods . . . 116

6.3 Total number of fibre strength results determined for each gauge length . . 118

6.4 Mean, median and mode values of fibre diameters for the different gauge lengths . . . 119

6.5 Mean, standard deviation and coefficient of variation (CoV) of the average Young’s modulus for tests done at the three gauge lengths . . . 125

6.6 Maximum likelihood parameters for the 2-parameter Weibull distribution . 129 6.7 Maximum likelihood parameters for the 3-parameter Weibull distribution . 130 6.8 Effect of sample size on the confidence interval of the median strength of the simulated fibre strength data sets. . . 134

7.1 Truth table demonstrating the survival and failure of fibres to simulate the preselection effect. X represents a rejected point while O represents a selected point. . . 141

*7.2 Relationship between location parameter (σu) and truncation limit (σr*) for
*different values of ω. . . 145*

7.3 Single fibre tensile strength data set for a gauge length of 30 mm. . . 147

7.4 Parameters for standard Weibull distributions. . . 148

7.5 Parameters for truncated Weibull distributions for different cases. . . 150

7.6 Parameters for predicted Weibull distributions for the 3 cases. . . 152

**List of publications**

Parts of the work presented in this thesis have been disseminated through a number of
written publications and oral communications. These are listed below, as of January 2020.
**Peer-reviewed journal publications**

• F. Islam, S. Joann`es, S. Bucknell, Y. Leray, A. Bunsell, L. Laiarinandrasana,
“In-vestigation of tensile strength and dimensional variation of T700 carbon fibres using
*an improved experimental setup”, Journal of Reinforced Plastics and Composites,*
2020, 39 (3-4), 144-162.

• F. Islam, S. Joann`es, L. Laiarinandrasana, “Evaluation of critical parameters in
*ten-sile strength measurement of single fibres”, Journal of Composites Science. 2019, 3, 69.*
• S. Joann`es, F. Islam, L. Laiarinandrasana, “Uncertainty in fibre strength

*charac-terisation due to uncertainty in measurement and sampling randomness”, Applied*

*Composite Materials*, 2020, 27, 165-184.

• F. Islam, S. Joann`es, L. Laiarinandrasana, A. Bunsell, “Weibull analysis based on
*Bayesian approach to model the strength behaviour of brittle fibres”, (Under Review)*
**Refereed conference publications**

• F. Islam, S. Joann`es, L. Laiarinandrasana, “Propagation of uncertainty from
*con-stituents to structural assessments in composite strength modelling”, in 23rd *

*In-ternational Conference on Composites Structures (ICCS 23)*, September 1-4, 2020,

Porto, Portugal

• F. Islam, S. Joann`es, L. Laiarinandrasana, “Adaptation of Weibull analysis to
*repre-sent strength behaviour of brittle fibres”, in International Conference on Composite*

*Materials (ICCM-22)*, August 11-16, 2019, Melbourne, Australia

• A. Rajpurohit, F. Islam, S. Joann`es, S. Bucknell, V.Singery, L. Laiarinandrasana,
“Characterization and statistical analysis of fibre strength at various processing
*stages”, in International Conference on Composite Materials (ICCM-22), August*
11-16, 2019, Melbourne, Australia

• F. Islam, S. Joann`es, S. Bucknell, Y. Leray, A. Bunsell, L. Laiarinandrasana, “To-wards accurate and efficient single fibre characterization to better assess failure

14 LIST OF TABLES
*strength distribution”, in European Conference on Composite Materials *

*(ECCM-18)*, June 24-28, 2018, Athens, Greece

• F. Islam, S. Joann`es, S. Bucknell, Y. Leray, A. Bunsell, L. Laiarinandrasana,
“Im-provements in determination of carbon fibre strength distribution using automation
*and statistical data analysis”, in Fiber Society’s Spring 2018 Conference, June 12-14,*
2018, Tokyo, Japan

**Conference abstracts**

• M.P. Widjaja, F. Islam, S. Joann`es, A. Bunsell, G. Mair, “The effect of input
proper-ties on the predicted failure of a type IV composite pressure vessel using a multiscale
*model”, in FiBreMoD Conference, December 11-12 2019, Leuven, Belgium*

• R. J. Lunn, F. Islam, Y. Leray, S. Joann`es, S. Bucknell and D.M. Stringer,
“Fur-ther Insights into the Fatigue of Hair Fibres through Statistical Analysis and
*Rele-vance to Hair Care Applications”, in HairS‘19 Symposium, September 11-13, 2019,*
Schluchsee, Germany

• F. Islam, S. Joann`es, L. Laiarinandrasana, “Effect of uncertainty in
*characteriza-tion on the variability of fibre strength distribucharacteriza-tions”, in Internacharacteriza-tional Conference*

*on Recent Advancements in Composite Materials*, February 25-28, 2019, IIT-BHU,

Varanasi, India

**Preamble**

**Background and Motivation**

Fibre reinforced composite materials are used in load-bearing structural applications for the aerospace, automotive, transportation and energy industry. For such high performance and critical applications, there are risks of serious complications on failure. Material rupture or structural failure can result in catastrophic consequences. These applications therefore necessitate reliable structural health monitoring techniques for evaluating the damage tolerance and useful lifetime of the structures. These assessments can be assisted by computational strength and damage models, which should ideally be able to predict failure and useful life of these critical composite structures accurately.

Many complex computational models have been developed to simulate the failure processes in fibre reinforced composites which lead to the ultimate failure of structures. These models are used for predicting the failure strength and for the lifetime analysis of composite structures. Since the properties of composite materials are governed by the properties of their constituents and their interactions, the reliability of the model predictions is strongly dependent on the accuracy of the constituent properties used as input. Uncertainty in fibre or matrix properties may result in variability in the predicted strength and lifetime of composite structures. The reliability of model predictions thus depends upon a strong understanding of the constituent properties and any uncertainties associated with it. Any uncertainties in input data raises doubts on the strength and lifetime predicted by the models and restricts their reliability. Due to a lack of reliable structural assessment models, composite structures are still overdesigned to ensure safety, which negates the potential weight-saving benefits that can be achieved with fully optimized structures.

**Aims**

The overall aim of this thesis is to develop a better understanding of the constituent properties of fibre reinforced composites, i.e. the properties of fibres and matrix, and to improve their characterisation process. More accurate constituent properties will empower composite strength models to make reliable predictions for the behaviour and lifetime of composite structures.

16 CHAPTER 0. PREAMBLE

**FiBreMoD project**

FiBreMoD is a Marie Sklodowska-Curie Innovative Training Network (ITN) project which brings together universities, research centres and companies from different countries world-wide. The project aims to train 13 Early-Stage Researchers (ESRs) to become multi-talented and interdisciplinary researchers that will be highly coveted in the field of com-posites. The different academic and industrial partners in FiBreMoD include:

• Katholieke Universiteit Leuven (KUL), Leuven, Belgium

• Imperial College of Science and Technology, London, United-Kingdom • University of Southampton, Southampton, United-Kingdom

• Ecole des Mines de Paris (Mines ParisTech), Evry, France • Weizmann Institute of Science, Rehovot, Israel

• Bundesanstalt fur materialforschung und prufung (BAM), Berlin, Germany • Toyota Motor Europe (TME), Brussels, Belgium

• Siemens Industry Software NV, Leuven, Belgium • Chomarat Textiles Industries, Le Cheylard, France • Dia-Stron Ltd., Andover, United-Kingdom

**Thesis as part of the FiBreMoD project**

Limiting the climate change induced temperature increase to less than 2°C will require strong reductions in greenhouse gas emissions. Lightweight materials and fibre-reinforced composites in particular, are a key enabling technology to achieve this goal. Current com-posite applications are however strongly overdesigned due to a lack of reliable design tools and predictive models for their mechanical properties. The objectives of the FiBreMoD project is to develop and apply models to improve the design of composite structures made with continuous fibre materials. The final application is the design of high pressure vessels and automotive parts.

**Chapter 1**

**Introduction**

**Contents**

**1.1** **Structural applications of fibre reinforced composites** **. . . . .** **17**

**1.2** **Predictive models for fibre composites . . . .** **18**

1.2.1 Issues with model predictions . . . 18

**1.3** **Constituent properties: Input data for models . . . .** **19**

1.3.1 Fibre strength . . . 20

1.3.2 Matrix and interfacial properties . . . 22

**1.4** **Main objectives of the thesis** **. . . .** **23**

**1.5** **Thesis outline . . . .** **24**

**Chapter summary in French . . . .** **26**

**1.1**

**Structural applications of fibre reinforced composites**

Fibre reinforced composite materials have very strong structural capabilities, especially
when both mechanical performance and light weight are desired. They have benefits over
other structural materials such that for a given density, they possess higher stiffness and
strength. These materials also offer better impact and corrosion resistance, and possess
excellent weathering stability. These properties make them an ideal material to be used
for structural applications. They are thus widely used in critical load-bearing structures
for the aerospace, automotive, transportation and wind energy industry [1, 2], some of
which are shown in Figure 1.1. Just the pressure vessels and structural components for
the aerospace industry represent together about 40% by volume of the total composite
market [3].
In the transportation industry, composite pressure vessels are used for the storage and transportation of high pressure liquids and gases. Compressing hydrogen and natural gas and storing it within a pressure vessel is an efficient storage method in terms of energy density. In commercial aircrafts, the use of composite materials has seen a sharp increase since the 1990s. In the last two civilian aircrafts produced, composite materials make up half of the weight of the structure, with 53% of Airbus A350 XWB (2014) and 46% of

18 CHAPTER 1. INTRODUCTION

Figure 1.1: Some structural applications of fibre reinforced composite materials [4, 5, 6, 7]. Airbus A220 (2016) been made up of composite materials [8]. In the automotive industry, composites have mainly been used in expensive cars that are produced in limited volume such as Lamborghini’s Aventador and Tesla’s Roadster. However, the use of composites in high volume automotive production is gradually increasing with the BMW i3 being one of the first high volume cars made of composite materials. In the wind energy industry, composite materials are used typically in blades and nacelles of wind turbines. Renewable energy is the fastest growing energy source (7.6% p.a.). It is eventually expected to displace coal to become the single largest source of global power generation by 2040 [9, 10] and the use of structural composites is expected to continue its steep rise.

**Key aspects of designing composite structures**

In-service safety and reliable lifetime assessments are key challenges for high performance load-bearing applications and require great care to be taken during their design. The de-sign of composite material structures can be assisted by computational models for predict-ing their mechanical properties at both component and structural level. Critical structures such as composite pressure vessels which are used for the storage of hydrogen or other gases at high pressures require very accurate computational models, so that the predictions can be used with confidence in industrial applications [11].

**1.2**

**Predictive models for fibre composites**

The strength and damage behaviour of composite materials is inherently complex and thus predicting the mechanical behaviour of composite structures remains highly chal-lenging. Many ongoing studies of different composite material research groups are fo-cussed on developing computational composite strength and damage models to predict the mechanical behaviour of composite materials and structures leading to their lifetime assessment. Some of these models are mentioned here: (i) a multiscale finite-element sim-ulation method [12, 13] from Mines ParisTech, (ii) an analytical hierarchical scaling law for composite fibre bundles from Imperial College London [14], and (iii) direct numerical simulations of composite fibre bundles from KU Leuven [15]. These models were also compared in a recently conducted benchmarking exercise [16]. Detailed reviews of these and other models are available in literature [14, 17].

**1.2.1** **Issues with model predictions**

1.3. CONSTITUENT PROPERTIES: INPUT DATA FOR MODELS 19 by the different models were found to spread over a large range, thus suggesting the reason for the lack of confidence of industry in such models. These discrepancies were found to occur for many aspects of damage and failure, such as ultimate strength, failure strain, and clustering of fibre-breaks. Moreover, there were differences between the mechanical behaviour predicted by the models and that observed experimentally. The large spread in modelling predictions and deviation from experimental results can be linked to two main reasons:

• An incomplete understanding of the complex interaction between the fibres and matrix in fibre reinforced composites which governs their failure mechanism. • Lack of reliable constituent properties which are used as input for the models. There are several previous and ongoing studies for obtaining a better understanding of the failure mechanisms in fibre reinforced composites to improve the state-of-the-art models. However, obtaining representative constituent properties to be used as input for these models has received less attention. There are significant experimental and theoretical challenges in obtaining reliable input data, some of which are explained in the next sub-sections. There are also inherent variabilities in the properties of the constituents that lead to variability in the strength of the composite materials. There is a need for the mod-els to also address this variability to improve the reliability of the mechanical behaviour predicted by the models.

Due to the lack of reliable predictive models, composite components are still overdesigned which leads to larger and heavier parts along with sub-optimal structural performance.

**1.3**

**Constituent properties: Input data for models**

The mechanical behaviour of fibre reinforced composites is governed by the properties of its constituents, i.e. fibres and matrix, and on the interaction between them. In light of this understanding, longitudinal tensile strength models thus require information about two key concepts: (i) the fibre strength distribution (ii) stress concentration around broken fibres. The stress concentration depends upon the properties of the matrix material and of the fibre-matrix interface. The properties of the fibres, matrix and the interface are together used as input in these models for evaluating the damage and failure behaviour of the composite structures [19].

20 CHAPTER 1. INTRODUCTION increased by a factor of ten on decreasing the standard deviation of input fibre strength distribution to a third of its initial value. It is therefore crucial for the success of composite strength models that the fibre, matrix and interfacial properties used as model input are determined with the best possible accuracy and any associated uncertainty is quantified appropriately.

The major input properties which are used by the models and the issues in accurately determining them are discussed in the next subsections.

**1.3.1** **Fibre strength**

There is a large variation in the strength of fibres and therefore their strength cannot be represented by a single average value. Fibre strength is typically represented by using statistical distribution functions, of which the Weibull distribution is the most popular. Weibull proposed a distribution that addresses the variation in strength of brittle fibres and could be used to represent their strength behaviour [23]. Many studies have proposed mod-ifications to this distribution for representing fibre strength but the standard 2-parameter Weibull probability distribution function given by Equation 1.1 has been the most widely used representation. In this equation, it is assumed that the section of the fibre remains constant along its length, the scope for which will be discussed in the forthcoming chapters.

*P*R*(σ) = 1 − exp*
−
_{L}*L*0
_{σ}*σ*0
*m*
(1.1)
*where, P*R*(σ) is the probability of fibre failure for an applied stress level σ, L being the*

*characteristic gauge length, L*0 *the reference gauge length, σ*0 *the scale parameter, m the*

*shape parameter or Weibull modulus. The scale parameter, σ*0, represents the strength

*at which 63.2% of the fibres within a population would fail. The shape parameter, m,*
represents the scatter in strength around the mean value. Fibre strengths are typically
reported in terms of the Weibull shape and scale parameters. These parameters are also fed
into the composite strength models, and are one of the most important input properties.
**Issues with fibre strength data**

On analysing the fibre strength properties available in literature, it has been observed
that there are differences in results reported by different authors, even for the same type
of fibres. For T700 carbon fibres, which are very popular in fibre reinforced composites
*for structural applications, the Weibull distribution parameters (m and σ*0) for the tensile

*strength reported by different studies are compiled in Table 1.1. The scale parameter σ*0,

depends on the gauge length used, so all reported scale parameter values have also been
*normalised for a gauge length of L*0 = 30 mm using the widely used Weibull scaling

*equation given by Equation 1.2, which is derived from Equation 1.1. σ0,1* *and σ0,2* are

*scale parameter values determined for fibre gauge lengths of L0,1* *and L0,2*, respectively

1.3. CONSTITUENT PROPERTIES: INPUT DATA FOR MODELS 21 estimating the strength of fibres will be discussed in later chapters.

*σ0,2* *= σ0,1*
*L0,1*
*L0,2*

!*1/m*

(1.2)
Table 1.1: Weibull distribution parameters for T700 carbon fibres reported in literature.
*The scale parameter (σ*0*) normalized for L*0 = 30 mm. ‘SFT’ stands for single fibre tests,

‘Fragm.’ stands for fibre fragmentation tests, and ‘Bundle’ stands for fibre bundle tests.

S.N. Type_{of fibre} Testing_{method} Gauge_{length} Sample_{size, N} Shape,* _{m}* Scale,

_{σ}0
*Scale, σ*0
(Norm.) Author
(mm) (GPa) (GPa)
1 T700 SFT 20 30 5.6 5.4 5.02 Feih [27]
2 T700 SFT 20 30 5.39 - - Hao [28]
3 T700 SFT
10 20 3.5 7.7 5.63
Deng [29]
20 20 5 6.2 5.72
30 20 4 6.2 6.20
40 20 3.7 6 6.49
50 20 4 5.8 6.59
4 T700 SFT 20 10 4.68 3.63 2.87 Lutz [30]
5 T700 SFT 10 20 12.01 3.92 3.58 Na [31]
6 T700 Fragm. 30 6 4.8 8.5 8.50 Deng [29]
7 T700 Fragm. 20 - 5.6 5.47 - Matveev [32]
8 T700 Bundle 20 15 17.53 1.98 1.93 Ting [33]
9 T700 Bundle 8 - 12.06 4.41 3.95 Zhou [34]

Figure 1.2(a) shows the scatter in the shape parameter values for different gauge lengths as reported by different authors, while Figure 1.2(b) shows the scale parameter values, nor-malised for a gauge length of 30 mm. Since different studies have used different method-ologies for determining the fibre strength distribution, results obtained from the different processes are represented by different geometric shapes in the plot. Values determined by using the single fibre testing (SFT) methodology are depicted with a circle and the size of the circles are in proportion to the sample size that was used to determine these results, as also given in Table 1.1. Values determined by using the fragmentation and bundle testing methodologies are depicted by diamond and square shaped markers, re-spectively. The shape parameter is observed to vary between 3.5-17.5 which is a huge variation. The normalised scale parameter values are also observed to have a big variation and lie between 1.9-8.5 GPa.

22 CHAPTER 1. INTRODUCTION

Figure 1.2: Weibull parameter values for T700 carbon fibres reported in literature for: a) Shape parameter b) Scale parameter. Circular, diamond and square-shaped markers represent results from the single fibre tests (SFT), fibre fragmentation tests and fibre bundle tests, respectively. The scale parameter values have been normalised for a gauge length of 30 mm using the Weibull scaling equation (Equation 1.2). The values originally reported are also shown.

that there is possibility of uncertainty in results [35], the exact causes of uncertainties and their effects on fibre strength results have not been investigated in detail.

**1.3.2** **Matrix and interfacial properties**

After fibre strength, the second key aspect for any strength model is the stress redistribu-tion around fibre breaks under longitudinal loading. When a fibre breaks, the surrounding matrix is subjected to a multi-axial stress state. This leads to an increase in the stress of the surrounding fibres, which is often described in terms of stress concentration factors (SCFs). The magnitude of stress concentrations is governed by the matrix and interfacial properties.

Matrix properties such as stiffness and strength contribute to the longitudinal tensile strength of composites. Whether the matrix has a perfectly elastic, perfectly plastic, visco-elastic or visco-plastic nature can cause further complexities in the model.

1.4. MAIN OBJECTIVES OF THE THESIS 23
**Issues with matrix and interfacial property data**

Most matrix systems have complex behaviour, i.e. they are not linearly elastic, but visco-elastic materials. Most models however have simplified this behaviour by treating the matrix as perfectly elastic or perfectly plastic. Moreover, matrix properties which deter-mine the fibre-matrix debonding are often very challenging to be measured. Many strength models in the literature even ignore debonding altogether.

More importantly, the matrix properties used as input data for strength models are always measured on macroscale specimens. However, some studies have suggested that it is very likely that the macroscale matrix behaviour is different from that at the microscale. This can result in significant differences between the model predictions and the mechanical behaviour of an actual composite material. A new method for characterizing the microscale properties of the matrix will be introduced in this thesis.

**1.4**

**Main objectives of the thesis**

It is evident that accurate input constituent properties are important for the success of composite strength models in determining reliable results. However, it has been shown that there is discrepancy in available constituent properties, mainly in the fibre strength distribution; and even for the same type of fibre, different studies have reported different results [26]. This makes the selection of input data for composite models ambiguous and also raises doubts on the reliability of the model predictions.

The main objective of this thesis is to develop a better understanding of the constituent properties of fibre reinforced composites. The discrepancy or variation in reported con-stituent properties could be due to a combination of many factors, as characterizing the properties of the constituents can be challenging. Some factors that can result in inaccurate characterisation are: measurement uncertainty, experimental errors, non-representativeness of the chosen sample set for data generation and analysis, the data-reduction technique used, etc. The effects of these factors need to be investigated to obtain a better understanding of the uncertainty associated with the constituent proper-ties, and to find the causes behind these uncertainties.

Since fibres are the principal load bearing constituents of unidirectional composites, most of the research described in this thesis deals with fibres, in order to understand and improve their characterisation process, by identifying and discriminating between different causes of uncertainties. The knowledge of the causes behind uncertainties can enable appropriate measures to be taken in order improve the characterisation of constituent properties by appropriately tackling the underlying causes.

To achieve the mentioned objectives, the following research will be described in this thesis: • Investigation of the variation in tensile strength and morphology of structural fibres • Identification and evaluation of critical parameters which contribute to errors in fibre

strength measurement

24 CHAPTER 1. INTRODUCTION • Simulating the effect of uncertainty in input properties on the variability of composite

model predictions

• Formulation of an improved data reduction technique to model the statistical vari-ation in strength of brittle fibres

**1.5**

**Thesis outline**

With an objective of understanding and improving the fibre strength characterisation process, Chapter 2 discusses the state-of-the-art. It includes analysis of major issues and challenges associated with different characterisation techniques, and with the Weibull disribution which is used to represent fibre strength behaviour.

In Chapter 3, different possible sources of errors due to experimental limitations in the single fibre testing process have been identified. Their effect on fibre tensile strength has been analytically modelled. This model is then used to evaluate the uncertainty in experimentally determined fibre strength at different gauge lengths.

Chapter 4 uses uncertainty in fibre strength calculated in Chapter 3 to determine its effects on the fibre strength distribution using a statistical Monte-Carlo method. These results are also analysed to elucidate the effect of sampling on the results.

The understanding of uncertainty in fibre strength distributions gained from Chapters 3 and 4 is then used to find its effect on the structural behaviour predictions of composite strength models. This study is described in Chapter 5.

To minimise uncertainties in fibre strength distribution, analysis of a large data set of ex-perimental results generated for a wide range of fibre gauge lengths is discussed in Chap-ter 6, so as to highlight the limitations of the standard Weibull analysis for representing fibre strength behaviour. The role of fibre dimensions on the fibre strength distribution is also discussed in this chapter.

In Chapter 7, the standard Weibull analysis has been adapted based on the Bayesian approach of using prior knowledge of how fibres break during the testing process. Fibre strength data is then analysed using this method to predict a more accurate statistical representation of the tensile strength behaviour of fibres used in composites.

1.5. THESIS OUTLINE 25

### Graphical Outline

### 1

### 7

### 6

### 5

### 4

### 3

### 2

*Does uncertainty in individual fibre strength affect the distribution ? *

- Identification of critical parameters - Uncertainty in measured fibre strength

- Uncertainty due to measurement errors is small - Uncertainty due to sampling randomness is large

Failure strength and lifetime of composite structures significantly affected

- By using a large sample data set for analysis

- Standard Weibull analysis is inappropriate for modelling

Formulation of a Weibull analysis based on Bayesian approach of using prior knowledge of how fibres break Discrepancy in input data for composite strength models

Issues with characterisation of fibre properties

*How to improve fibre strength characterisation ? *
*Why ? *

*Does uncertain input data affect composite model predictions ? *

*How can uncertainty in Weibull parameters be minimised ? *

*How to accurately model the true fibre strength behaviour ? *

Conclusions and Perspectives

### 8

26 CHAPTER 1. INTRODUCTION

**Chapter summary in French**

**Introduction**

*Les mat´eriaux composites renforc´es de fibres ont de tr`es fortes capacit´es structurelles, en*
*particulier lorsque des performances m´ecaniques associ´ees `a un poids l´eger sont recherch´es.*
*Ils sont donc largement utilis´es dans les structures porteuses critiques pour l’industrie*
*a´erospatiale, a´eronautique, automobile et de l’´energie ´eolienne. La s´ecurit´e en service et les*
*´evaluations fiables de la dur´ee de vie sont des d´efis cl´es pour les applications structurelles*
*hautes performances et n´ecessitent un grand soin lors de leur conception. La conception*
*de structures en mat´eriaux composites peut ˆetre assist´ee par des mod`eles pour pr´edire leurs*
*propri´et´es m´ecaniques au niveau des composants et de la structure. De nombreux mod`eles*
*proposent des solutions pour pr´edire au mieux la r´esistance des structures composites en*
*se basant g´en´eralement sur les m´ecanismes d’endommagement intervenant au cœur du*
*mat´eriau.*

*Afin d’´evaluer les pr´evisions faites par ces mod`eles, des exercices d’analyses comparatives*
*de leurs performances ont ´et´e men´es dans le monde. Il a ´et´e constat´e que les pr´evisions*
*faites par les diff´erents mod`eles s’´etalaient sur une large gamme de valeurs, entraˆınant un*
*manque de confiance de l’industrie dans ces mod`eles. Il existe de nombreuses ´etudes visant*
*`*

*a obtenir une meilleure compr´ehension des m´ecanismes de d´efaillance dans les *
*compos-ites renforc´es de fibres et ceci afin d’am´eliorer les mod`eles existants. Un autre probl`eme*
*provient de l’obtention des propri´et´es des constituants, variables d’entr´ee de ces mod`eles.*
*Il existe d’importants d´efis exp´erimentaux et th´eoriques pour obtenir des donn´ees d’entr´ee*
*fiables. Il existe ´egalement des variabilit´es inh´erentes aux propri´et´es des constituants qui*
*conduisent `a une variabilit´e de la r´esistance des mat´eriaux composites. Il est n´ecessaire*
*que les mod`eles tiennent ´egalement compte de cette variabilit´e pour am´eliorer la fiabilit´e*
*du comportement m´ecanique pr´edit.*

*En analysant les propri´et´es de r´esistance des fibres disponibles dans la litt´erature, il a*
*´et´e observ´e qu’il existe des diff´erences dans les r´esultats rapport´es par diff´erents auteurs,*
*mˆeme pour le mˆeme type de fibres. Les param`etres de la distribution de Weibull pour les*
*fibres de carbone T700, qui sont tr`es populaires dans les composites pour les applications*
*structurelles, sont discut´es dans ce chapitre et une grande dispersion a ´et´e observ´ee.*
*Dans le but d’am´eliorer la compr´ehension des propri´et´es constitutives des composites *
*ren-forc´es de fibres, les recherches suivantes seront d´ecrites dans cette th`ese:*

*• Etude de la variation de la r´esistance `a la traction et de la morphologie des fibres*

*structurales*

*• Identification et ´evaluation des param`etres critiques qui contribuent aux erreurs de*

*mesure de la r´esistance des fibres*

*• Quantification statistique de l’incertitude des param`etres de distribution de la r´esistance*

*des fibres*

*• Simulation de la cons´equence de l’incertitude des propri´et´es d’entr´ee sur la variabilit´e*

*des pr´edictions du mod`ele `a l’´echelle du composite*

1.5. THESIS OUTLINE 27

*variation statistique de la r´esistance des fibresfragiles*

**Chapter 2**

**Fibre strength and Weibull**

**distribution: state-of-the-art**

**Contents**

**2.1** **Introduction** **. . . .** **29**

2.1.1 Fibres used in composite materials . . . 30

**2.2** **Fibre strength** **. . . .** **31**

2.2.1 Weakest link model for fibre strength . . . 31 2.2.2 Representation of fibre strength with Weibull distribution . . . . 32 2.2.3 Physical interpretation of Weibull distribution parameters . . . . 33

**2.3** **Fibre strength characterisation . . . .** **33**

2.3.1 Fibre bundle test . . . 35 2.3.2 Fragmentation test . . . 36 2.3.3 Loop test . . . 37 2.3.4 Single fibre test . . . 38 2.3.5 Estimation of Weibull parameters from fibre strength data set . . 40

**2.4** **Issues in determining fibre strength . . . .** **41**

**2.5** **Issues with the standard Weibull distribution . . . .** **42**

2.5.1 Extrapolation of distribution parameters . . . 42 2.5.2 Discrepancy between experimental results and Weibull model . . 42 2.5.3 Uncertainty in results . . . 43

**2.6** **Conclusions . . . .** **44**

**Chapter summary in French . . . .** **46**

**2.1**

**Introduction**

Fibres are known to be an essential constituent of many living things. They are present in nanostructures such as twisted strands of DNA and also in large and complex struc-tures such as the muscles and tissues of both mammals and trees. Humankind has taken

30 CHAPTER 2. STATE-OF-THE-ART inspiration from such structures to use fibres for the development of textile materials and fibre-reinforced composites. Fibres are widely used in composite materials to make light-weight and high-strength products. The reinforcement of polymeric matrices by fibres is found to bring about significant advancements in the mechanical behaviour of polymers. This provides added advantages such as high strength to weight ratio, excellent weathering stabilities and enhanced dimensional stabilities. This combination can generate some of the strongest and versatile materials that have ever been known or developed.

Most outstanding characteristics of composite materials are imparted by the fibres which are used to reinforce the matrix, as these fibres are the principal load bearing constituents of unidirectional composite materials. Failure of composite materials typically occurs due to the accumulation of fibre breaks. Knowledge of fibre strength is therefore crucial for understanding the failure behaviour of fibre reinforced composite materials and structures. Using computational strength models, which uses the fibre properties as input, a simulation of the effective properties of the composite materials can be made, enabling an estimation of failure onset [11, 12, 13, 15, 36].

Matter in the form of fibres is capable of possessing extraordinary properties of strength and stiffness. Fibres do not share the properties with the same material in bulk form, whilst some fibres do not even exist in bulk form. For e.g. Glass fibres can be hundreds of times stronger than glass in bulk form. This is because there are far fewer defects in fine fibres as compared to the bulk state. Therefore, an assembly of fibres making up the same volume as that in bulk form would be much stronger. This is also true for other materials. It is however important to note that this is true when the strength is considered in a direction parallel to the fibres in the fibre assembly. The fibre assembly is anisotropic unlike the case for the bulk material which has the same characteristics in all directions and is therefore isotropic.

**2.1.1** **Fibres used in composite materials**

Different fibres are used as reinforcements in composite materials. The desired
character-istics of most reinforcing fibres are high strength, high stiffness, and low density. Some
commonly used fibres in composite materials are made of: Carbon, Glass, Aramid, Boron,
**etc. Carbon fibres are most widely used for advanced composites. They are available in**
**many forms with a range of stiffness and strengths. Glass fibres are commonly used in**
low to medium performance composites, due to their high tensile strength and low cost.
They are usually not used for very high performance applications because of their
rela-tively low stiffness, and they are also prone to degradation in properties with exposure
**to hygrothermal conditions. Aramid (or Kevlar) fibres have relatively higher stiffness**
than glass fibres. Morover, they have low density, high tensile strength, and good impact
resistance and toughness. However, Kevlar composites have very low transverse tensile
and longitudinal compressive strengths. They are also very sensitive to moisture
**absorp-tion. Boron and other ceramic fibres typically have high stiffness and strength, and high**
use temperatures. They are usually used in high temperature applications with metal
or ceramic matrices. Figure 2.1 shows rovings of some fibre types used in composite
materials.

2.2. FIBRE STRENGTH 31

Figure 2.1: Rovings of some fibre types used in composite materials [37]. (a) Carbon (b) Glass (c) Aramid.

applications, for example in pressure vessels and aircraft components. For the rest of the thesis, most of the reviews, analysis, and concepts developed will be demonstrated using carbon fibres and their composites. Nevertheless, these concepts and theories are also applicable to other brittle fibres as well.

**2.2**

**Fibre strength**

The “strength” of a structure is defined as its ability to withstand an applied load without breaking. For a given single fibre, to assess its strength, a monotonic longitudinal load is applied to the fibre until its failure. This failure load is then normalized by the cross-section, possibly at the breaking point, to obtain the tensile strength of the fibre.

As mentioned by Timoshenko, Leonardo da Vinci was the first to study the strength of materials as a function of their size, when he demonstrated in the 1500s, that longer iron wires are weaker than shorter ones [38]. A major advancement was made by made by Mariotte in 1686, when he experimented with ropes and concluded that, “a long rope and a short one always support the same weight unless that in a long rope there may happen to be some faulty place in which it will break sooner than in a shorter”. Griffiths later explained this size dependency of strength based on the presence of flaws. Since a shorter fibre has a lower probability of having a flaw, it is more likely to have a higher strength. This reasoning also represented a physical basis of Da Vinci’s and Mariotte’s qualitative observations. Further investigations on size effects were made by Tipett (1925), Peirce (1926) and Frechet (1927). This progress culminated with the work of Weibull in 1939 [39, 40].

**2.2.1** **Weakest link model for fibre strength**

32 CHAPTER 2. STATE-OF-THE-ART to the distribution of defects in the volume or on the surface of fibres. The theoretical description of the weakest link model for representing fibre strength, as also demonstrated by Weibull, is described in Appendix A.

Figure 2.2: Schematic representation of a chain consisting of N links. The chain breaks at the weakest link.

**2.2.2** **Representation of fibre strength with Weibull distribution**

Technical fibres used as reinforcements in organic matrix composite materials are usually
brittle in nature. Strengths of brittle fibres such as carbon and glass are controlled by
the stochastic distribution of defects inside them, due to which there are variations in
the strength of individual fibres. Fibre strength, therefore, cannot be described by a
single value and is typically represented by using a statistical function which characterizes
the inherent variation in its strength. The most popularly used statistical function for
representing strength of brittle fibres is the Weibull distribution [23]. The weakest link
model outlined above, and detailed in Appendix A, was used as a basis by Weibull to
represent the behaviour of a brittle solid for which failure of the material is induced due
to the presence of a crack, developed from the most critical defect. The parameters of
the Weibull distribution characterises the strength variation of fibres and are determined
by appropriately fitting experimentally generated fibre strength data with the statistical
function. The failure probability of a fibre, following the Weibull law, can be expressed
as in Equation 2.1, which is popularly known as the 3-parameter Weibull distribution.
*For fibres of uniform cross-sections, the term V/V*0 *can be replaced by L/L*0, as shown

in Equation 2.2.
*P*R*(σ) = 1 − exp*
−
_{V}*V*0
_{σ − σ}*u*
*σ*0
*m*
*,* *for σ ≥ σu* (2.1)
*PR(σ) = 1 − exp*
−
_{L}*L0*
_{σ − σ}*u*
*σ0*
*m*
*,* *for σ ≥ σu* (2.2)
*with P*R*(σ) = 0 for σ < σu*.

*Here, P*R*(σ) is the probability of fibre failure, L the characteristic gauge length, (V being*

*the characteristic gauge volume), L*0 *the reference gauge length, (V*0 being the reference

*gauge volume), σ the applied stress, σu* *the location parameter, σ*0 the scale parameter,
*m* *the shape parameter or Weibull modulus. The shape parameter (m) describes the*

range of variation in fibre strength data, i.e. the scatter around an average value, the
*scale parameter (σ*0) is the 63.2 percentile strength value of the distribution and the

*location parameter (σu*) determines the starting point or the origin of the distribution.

2.3. FIBRE STRENGTH CHARACTERISATION 33
*different gauge lengths to a common reference length (L*0), and for extrapolating the scale

parameter to other lengths, to account for the length effect [41].

When an experimentally determined fibre strength data set is analysed with this
distribu-tion, the best fitted distribution originates around the point of the smallest strength value
in the data set. This determines the location parameter which which represents the origin.
It has also been called as the threshold parameter by some authors. Most studies have
*chosen to fix this location parameter σu* to be zero. This results in a 2-parameter

distribu-tion which originates at zero strength value, and is given by Equadistribu-tion 2.3 or Equadistribu-tion 2.4, for the cases of non-uniform and uniform cross-sections, respectively. Equation 2.4 is also the most popularly used function for representing the strength behaviour of brittle fibres [26]. The limitations of using either of the 2 or 3-parameter Weibull distribution for representing the fibre strength behaviour would be discussed in another chapter.

*P*R*(σ) = 1 − exp*
−
_{V}*V*0
_{σ}*σ*0
*m*
(2.3)
*P*R*(σ) = 1 − exp*
−
_{L}*L*0
_{σ}*σ*0
*m*
(2.4)
**2.2.3** **Physical interpretation of Weibull distribution parameters**

*The effects of varying the shape (m), scale (σ*0*) and location (σu*) parameters on the

resulting Weibull distribution is shown in Figure 2.3. These distributions have been obtained by varying one of the three parameters of the Weibull distribution, while fixing the other two. Figure 2.3(a) shows the effect of varying the shape parameter, Figure 2.3(b) shows the effect of varying the scale parameter, while Figure 2.3(c) shows the effect of varying the location parameter, on the resulting distributions. It should however be noted that these parameters of the Weibull distribution are not independent of each other and variations in the value of one parameter leads to variations in the values of the other parameters as well.

**2.3**

**Fibre strength characterisation**

Characterizing fibres is challenging, as the fibre diameter can be just a few microns es-pecially for brittle technical fibres such as carbon. The very small cross-section of fibres makes them very delicate to handle leading to a very cumbersome process of fibre speci-men preparation and testing [42]. These challenges significantly affect the accuracy of the prepared specimen and may lead to inaccurate fibre strength measurements [26, 35, 43]. Despite considerable progress in characterisation techniques, many obstacles still remain to obtain accurate fibre strength data.

34 CHAPTER 2. STATE-OF-THE-ART

*(a) Effect of shape parameter (m)* *(b) Effect of scale parameter (σ*0)

*(c) Effect of location parameter (σu*)

*Figure 2.3: Effects of the shape (m), scale (σ*0*) and location parameters (σu*) on Weibull

2.3. FIBRE STRENGTH CHARACTERISATION 35 determine the parameters for the fibre strength distribution. The single fibre test is one of the most straightforward techniques however; it is a very laborious and time consuming process. The next subsections discuss these available techniques for the determination of fibre strength distribution, along with the challenges that are associated with each methodology.

**2.3.1** **Fibre bundle test**

In fibre bundle tests, a bundle containing a large number of fibres is subjected to tensile
*loading and the load-strain curve is recorded. The load F and applied strain ε are then*
represented using an appropriate form of a Weibull distribution given by Equation 2.5, as
discussed previously by a number of authors [44, 45, 46]. It is assumed that all fibres in
the bundle are nominally identical, that they are perfectly aligned and are linear elastic
in nature.
*F* *= Ebε*exp
−*l*
*l*0
_{ε}*βε*
*α*
(2.5)
*where Eb* *= AEN*0*, A is the single fibre cross-sectional area, E the modulus, N*0 the

*number of fibres in the bundle, l the bundle gauge length, l*0 the bundle gauge length,
*α* *the shape parameter, and βε* *is related to the scale parameter β as βε= β/E.*

**Limitations:**

• The analysis is based on the assumption of equal load sharing amongst the surviving
fibres of identical length. However, the spread of the individual fibre gauge length
inside the bundle is unavoidable which may lead to unequal distribution of stress on
the fibres. It has been shown that there may be a difference in the bundle length
*and fibre length. This difference, called slack, ϕ, introduces a non-linearity in the*
load-strain curve [47, 48] as shown in Figure 2.4.

36 CHAPTER 2. STATE-OF-THE-ART • The fibres inside a bundle interact laterally with each other. This causes local

shearing and contributes to the fibres adjacent to breaks [49, 50].

• When considering load transfer interactions, most strength models for fibre-reinforced composites use the idea that the entire surface area of each fibre is surrounded by the matrix material. Load transfer within the composite is then achieved through each individual fibre-matrix interaction, instead of through the interaction between a group of fibres and the matrix, as in fibre bundle test results.

• Depending upon the type of material and manufacturing process used for making the fibres, there can be significant variations in diameter of different fibres and in some cases, along the length as well. Due to this non-uniformity in fibre dimensions, the bundle test may not be a very appropriate method to determine fibre strength distribution.

**2.3.2** **Fragmentation test**

In this method, a single fibre is embedded in a matrix and the composite is subjected to a longitudinal incremental displacement. The fibre inside the matrix breaks repeat-edly at different locations along the length of the fibre, as demonstrated in the schematic in Figure 2.5. Polarized light is used to identify the sites of fibre breaks. Ultimately, a saturation point is reached when there are no further fibre breaks and there are a very large number of very short fibre segments. The number of fibre breaks is inspected contin-uously and is deduced to be a function of the applied load, until the onset of saturation. At each break, the corresponding stress is recorded, and the average fragment length is calculated. The Weibull shape and scale parameters are obtained from Equation 2.6. This methodology has been described by different authors [51, 52, 53, 54].

2.3. FIBRE STRENGTH CHARACTERISATION 37
*σf* *= αL*(−
1
*β*)Γ
1 +1
*β*
(2.6)
*where L is the average fibre length, σf* *is applied stress, α and β are Weibull scale and*

shape parameters, respectively and Γ is the Gamma function.
**Limitations:**

• If the bonding at the interface of fibre and matrix is too strong, the fibre cracks may propagate into the matrix and cause the matrix to deform around the crack. On the other hand, if the bonding at the interface is weak, debonding between the matrix and fibre may occur which may result in the fibre slipping out of the matrix. This may change the gap between broken fibres and hamper load transfer to the remaining parts of the fibre [55].

• The theory of fragmentation requires that the fragmentation data is strictly log-normally distributed. It has also been found in different studies that the fibre frag-ment length distribution indeed follows a log-normal distribution, but only in the early fragmentation stages [51, 56].

• The calculation of fibre stress can be affected by residual stresses developed due to different rates of thermal expansions in fibres and matrix. It has been shown that the Weibull parameters can be very sensitive to residual stresses [54, 57]. For calibrating the fibre stresses, residual stresses need to be determined by comparing the fibre stress calculated using fragmentation tests to the stresses calculated from single fibre tests. Alternatively, it can be estimated using a method proposed by Tsai [58].

• It is assumed that fibre breaks are non-interacting in nature. This assumption is only valid if the fibre break density is very low. Several models have been developed to capture the effect of fibre break interactions [52, 59, 60, 61], some of which add a parameter called exclusion zone length [62]. However, such models are very sensitive to the stress transfer between matrix and fibres requiring very accurate information about the exclusion zone length; determining which is complex and it may also vary with fibre stress.

**2.3.3** **Loop test**